#------------------------------------------------------------------------------
#$Date: 2023-11-06 09:25:17 +0200 (Mon, 06 Nov 2023) $
#$Revision: 287339 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/24/74/7247470.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7247470
loop_
_publ_author_name
'Poręba, Tomasz'
'Świątkowski, Marcin'
'Confalonieri, Giorgia'
_publ_section_title
;
 Melting pseudosymmetry and thermal expansion in 3-benzoylpropionic acid
;
_journal_issue                   42
_journal_name_full               CrystEngComm
_journal_page_first              5932
_journal_page_last               5941
_journal_paper_doi               10.1039/D3CE00940H
_journal_volume                  25
_journal_year                    2023
_chemical_formula_moiety         'C10 H10 O3'
_chemical_formula_sum            'C10 H10 O3'
_chemical_formula_weight         178.18
_chemical_name_common            '3-benzoylpropionic acid'
_chemical_name_systematic        '3-benzoylpropionic acid'
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2yn'
_space_group_name_H-M_alt        'P 1 21/n 1'
_atom_sites_solution_hydrogens   difmap
_audit_creation_date             2023-06-07
_audit_creation_method
;
Olex2 1.5
(compiled 2023.03.06 svn.rbb2c1857 for OlexSys, GUI svn.r6748)
;
_audit_update_record
;
2023-07-20 deposited with the CCDC.	2023-10-04 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 111.513(4)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   12.8072(4)
_cell_length_b                   5.24245(15)
_cell_length_c                   14.4951(4)
_cell_measurement_reflns_used    5197
_cell_measurement_temperature    279.99(10)
_cell_measurement_theta_max      78.4970
_cell_measurement_theta_min      3.9400
_cell_volume                     905.42(5)
_computing_cell_refinement       'CrysAlisPro 1.171.42.68a (Rigaku OD, 2022)'
_computing_data_collection       'CrysAlisPro 1.171.42.68a (Rigaku OD, 2022)'
_computing_data_reduction        'CrysAlisPro 1.171.42.68a (Rigaku OD, 2022)'
_computing_molecular_graphics    'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2017/1 (Sheldrick, 2015)'
_diffrn_ambient_environment      air
_diffrn_ambient_temperature      279.99(10)
_diffrn_detector                 'Hybrid Pixel Array Detector'
_diffrn_detector_area_resol_mean 5.8140
_diffrn_detector_type            'Pilatus 300K'
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.953
_diffrn_measurement_details
;
List of Runs (angles in degrees, time in seconds):

  # Type    Start    End  Width  tₑₓₚ   ω     θ     κ     φ   Frames
#--------------------------------------------------------------------------
  1  ω    -26.00  27.00   0.50    0.50    --  -49.12  19.00 -60.00  106
  2  ω   -120.00 -41.00   0.50    0.50    --  -49.12-178.00 -90.00  158
  3  ω    -26.00  27.00   0.50    0.50    --  -49.12  19.00 -30.00  106
  4  ω    -26.00  27.00   0.50    0.50    --  -49.12  19.00   0.00  106
  5  ω    -23.00 121.00   0.50    0.50    --   49.12   0.00 -90.00  288
  6  ω     62.00 120.00   0.50    0.50    --   49.12 178.00 -30.00  116
  7  ω    -43.00 -13.00   0.50    2.50    --  -88.50  38.00 -60.00   60
  8  ω    -43.00 -13.00   0.50    2.50    --  -88.50  38.00 -30.00   60
  9  ω    -43.00 -13.00   0.50    2.50    --  -88.50  38.00   0.00   60
 10  ω    -43.00 -13.00   0.50    2.50    --  -88.50  38.00  30.00   60
 11  ω    -43.00 -13.00   0.50    2.50    --  -88.50  38.00 150.00   60
 12  ω   -160.00 -73.00   0.50    2.50    --  -88.50 -57.00-150.00  174
 13  ω     38.00  66.00   0.50    2.50    --  110.00 -57.00 -90.00   56
 14  ω     97.00 178.00   0.50    2.50    --  110.00  19.00 150.00  162
 15  ω     38.00  66.00   0.50    2.50    --  110.00 -57.00 -30.00   56
 16  ω     98.00 178.00   0.50    2.50    --  110.00  38.00  30.00  160
 17  ω     38.00  66.00   0.50    2.50    --  110.00 -57.00 150.00   56
 18  ω     38.00  66.00   0.50    2.50    --  110.00 -57.00 -60.00   56
 19  ω     45.00 105.00   0.50    2.50    --  110.00 -77.00  90.00  120
 20  ω     38.00  66.00   0.50    2.50    --  110.00 -57.00   0.00   56
 21  ω     97.00 178.00   0.50    2.50    --  110.00  19.00  90.00  162
 22  ω     38.00  66.00   0.50    2.50    --  110.00 -57.00 120.00   56
 23  ω   -114.00 -25.00   0.50    0.50    --  -49.12 -77.00 -30.00  178
 24  ω     26.00 114.00   0.50    0.50    --   49.12  77.00-120.00  176
 25  ω     26.00 114.00   0.50    0.50    --   49.12  77.00  60.00  176
 26  ω     62.00 120.00   0.50    0.50    --   49.12 178.00-150.00  116
 27  ω     37.00 125.00   0.50    0.50    --   49.12  19.00  30.00  176
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'XtaLAB Synergy, Dualflex, Pilatus 300K'
_diffrn_measurement_method       'ω scans'
_diffrn_orient_matrix_type
'CrysAlisPro convention (1999,Acta A55,543-557)'
_diffrn_orient_matrix_UB_11      0.0562699000
_diffrn_orient_matrix_UB_12      -0.1802820000
_diffrn_orient_matrix_UB_13      0.0882307000
_diffrn_orient_matrix_UB_21      0.1140991000
_diffrn_orient_matrix_UB_22      0.0421685000
_diffrn_orient_matrix_UB_23      -0.0107104000
_diffrn_orient_matrix_UB_31      0.0233931000
_diffrn_orient_matrix_UB_32      0.2281537000
_diffrn_orient_matrix_UB_33      0.0717323000
_diffrn_radiation_monochromator  mirror
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Cu K\a'
_diffrn_radiation_wavelength     1.54184
_diffrn_reflns_av_R_equivalents  0.0377
_diffrn_reflns_av_unetI/netI     0.0272
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.953
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_k_max       6
_diffrn_reflns_limit_k_min       -5
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            9383
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.953
_diffrn_reflns_theta_full        67.684
_diffrn_reflns_theta_max         80.150
_diffrn_reflns_theta_min         3.948
_diffrn_source                   'micro-focus sealed X-ray tube'
_diffrn_source_type              'PhotonJet (Cu) X-ray Source'
_exptl_absorpt_coefficient_mu    0.803
_exptl_absorpt_correction_T_max  0.976
_exptl_absorpt_correction_T_min  0.821
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.42.68a (Rigaku Oxford Diffraction, 2022)
Analytical numeric absorption correction using a multifaceted crystal
model based on expressions derived by R.C. Clark & J.S. Reid.
(Clark, R. C. & Reid, J. S. (1995). Acta Cryst. A51, 887-897)
Empirical absorption correction using spherical harmonics,
implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            colourless
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    1.307
_exptl_crystal_description       plate
_exptl_crystal_F_000             376
_exptl_crystal_size_max          0.293
_exptl_crystal_size_mid          0.288
_exptl_crystal_size_min          0.03
_refine_diff_density_max         0.136
_refine_diff_density_min         -0.167
_refine_diff_density_rms         0.028
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.061
_refine_ls_hydrogen_treatment    refall
_refine_ls_matrix_type           full
_refine_ls_number_parameters     158
_refine_ls_number_reflns         1891
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.061
_refine_ls_R_factor_all          0.0516
_refine_ls_R_factor_gt           0.0436
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0574P)²+0.0899P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1207
_refine_ls_wR_factor_ref         0.1273
_reflns_Friedel_coverage         0.000
_reflns_number_gt                1520
_reflns_number_total             1891
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d3ce00940h2.cif
_cod_data_source_block           tp_bacidup_11_280_00
_cod_depositor_comments
'Adding full bibliography for 7247467--7247477.cif.'
_cod_database_code               7247470
_shelx_shelxl_version_number     2017/1
_chemical_oxdiff_formula         'C10 H10 O3'
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_max   0.976
_shelx_estimated_absorpt_t_min   0.799
_olex2_refinement_description
;
;
_olex2_submission_special_instructions 'No special instructions were received'
_oxdiff_exptl_absorpt_empirical_details
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
;
_oxdiff_exptl_absorpt_empirical_full_max 2.228
_oxdiff_exptl_absorpt_empirical_full_min 0.421
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, -y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
O3 O 0.65967(10) 0.4938(2) 0.47656(7) 0.0918(4) Uani 1 1 d . . . . .
O1 O 0.87553(10) 0.4946(3) 0.40579(9) 0.0997(4) Uani 1 1 d . . . . .
O2 O 0.93732(13) 0.7782(3) 0.52628(10) 0.1017(4) Uani 1 1 d . . . . .
C5 C 0.51866(11) 0.3522(3) 0.32977(9) 0.0632(3) Uani 1 1 d . . . . .
C4 C 0.61534(12) 0.5160(3) 0.38748(10) 0.0665(4) Uani 1 1 d . . . . .
C6 C 0.47087(14) 0.3588(3) 0.22689(10) 0.0766(4) Uani 1 1 d . . . . .
C1 C 0.86198(14) 0.6923(3) 0.44598(13) 0.0821(5) Uani 1 1 d . . . . .
C10 C 0.47539(13) 0.1827(4) 0.38015(12) 0.0815(5) Uani 1 1 d . . . . .
C3 C 0.65859(17) 0.7106(4) 0.33387(13) 0.0839(5) Uani 1 1 d . . . . .
C7 C 0.38368(15) 0.1989(4) 0.17647(13) 0.0916(6) Uani 1 1 d . . . . .
C2 C 0.75892(18) 0.8545(4) 0.40388(18) 0.0978(6) Uani 1 1 d . . . . .
C8 C 0.34331(16) 0.0287(4) 0.22723(16) 0.0987(6) Uani 1 1 d . . . . .
C9 C 0.38868(15) 0.0204(4) 0.32895(16) 0.0976(6) Uani 1 1 d . . . . .
H2 H 1.007(2) 0.675(5) 0.5475(19) 0.147(10) Uiso 1 1 d . . . . .
H3A H 0.5970(18) 0.825(4) 0.2959(14) 0.111(6) Uiso 1 1 d . . . . .
H3B H 0.6789(16) 0.613(4) 0.2861(14) 0.099(6) Uiso 1 1 d . . . . .
H6 H 0.5016(15) 0.478(3) 0.1954(12) 0.082(5) Uiso 1 1 d . . . . .
H10 H 0.5060(15) 0.186(3) 0.4476(14) 0.092(5) Uiso 1 1 d . . . . .
H7 H 0.3504(17) 0.210(4) 0.1069(16) 0.113(6) Uiso 1 1 d . . . . .
H8 H 0.281(2) -0.077(5) 0.1881(17) 0.130(8) Uiso 1 1 d . . . . .
H2A H 0.7465(17) 0.926(4) 0.4621(15) 0.108(6) Uiso 1 1 d . . . . .
H2B H 0.779(2) 0.998(5) 0.3719(16) 0.130(8) Uiso 1 1 d . . . . .
H9 H 0.363(2) -0.088(5) 0.3669(17) 0.132(8) Uiso 1 1 d . . . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0181 0.0091 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0492 0.0322 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_exptl_crystal_face_index_h
_exptl_crystal_face_index_k
_exptl_crystal_face_index_l
_exptl_crystal_face_perp_dist
2 -3 -2 0.1661
-2 3 2 0.1014
3 0 7 0.1463
-3 0 -7 0.1294
-7 0 7 0.0295
7 0 -7 0.0010
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
C1 O2 H2 112.3(15) . . ?
C6 C5 C4 122.53(14) . . ?
C10 C5 C4 118.98(12) . . ?
C10 C5 C6 118.48(14) . . ?
O3 C4 C5 120.84(13) . . ?
O3 C4 C3 119.88(14) . . ?
C5 C4 C3 119.27(12) . . ?
C5 C6 H6 116.1(10) . . ?
C7 C6 C5 120.55(17) . . ?
C7 C6 H6 123.4(10) . . ?
O1 C1 O2 122.12(18) . . ?
O1 C1 C2 122.70(16) . . ?
O2 C1 C2 115.15(16) . . ?
C5 C10 H10 117.0(12) . . ?
C9 C10 C5 120.65(16) . . ?
C9 C10 H10 122.4(12) . . ?
C4 C3 C2 111.96(15) . . ?
C4 C3 H3A 109.3(12) . . ?
C4 C3 H3B 104.9(11) . . ?
C2 C3 H3A 112.4(12) . . ?
C2 C3 H3B 110.9(11) . . ?
H3A C3 H3B 107.0(15) . . ?
C6 C7 H7 119.5(13) . . ?
C8 C7 C6 120.29(16) . . ?
C8 C7 H7 120.2(13) . . ?
C1 C2 C3 113.24(16) . . ?
C1 C2 H2A 105.1(12) . . ?
C1 C2 H2B 106.7(15) . . ?
C3 C2 H2A 113.5(12) . . ?
C3 C2 H2B 112.1(14) . . ?
H2A C2 H2B 105.6(18) . . ?
C7 C8 C9 120.14(18) . . ?
C7 C8 H8 116.9(14) . . ?
C9 C8 H8 122.9(14) . . ?
C10 C9 H9 116.6(15) . . ?
C8 C9 C10 119.9(2) . . ?
C8 C9 H9 123.5(15) . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
O3 C4 1.2106(16) . ?
O1 C1 1.2321(19) . ?
O2 C1 1.290(2) . ?
O2 H2 0.99(3) . ?
C5 C4 1.487(2) . ?
C5 C6 1.3893(18) . ?
C5 C10 1.388(2) . ?
C4 C3 1.506(2) . ?
C6 C7 1.373(3) . ?
C6 H6 0.940(17) . ?
C1 C2 1.499(3) . ?
C10 C9 1.380(2) . ?
C10 H10 0.911(18) . ?
C3 C2 1.514(3) . ?
C3 H3A 0.98(2) . ?
C3 H3B 0.97(2) . ?
C7 C8 1.372(3) . ?
C7 H7 0.94(2) . ?
C2 H2A 0.99(2) . ?
C2 H2B 0.97(3) . ?
C8 C9 1.373(3) . ?
C8 H8 0.97(3) . ?
C9 H9 0.93(3) . ?
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O3 C4 C3 C2 1.2(2) . . . . ?
O1 C1 C2 C3 22.0(3) . . . . ?
O2 C1 C2 C3 -159.81(16) . . . . ?
C5 C4 C3 C2 -178.45(14) . . . . ?
C5 C6 C7 C8 -0.6(3) . . . . ?
C5 C10 C9 C8 -1.0(3) . . . . ?
C4 C5 C6 C7 178.13(14) . . . . ?
C4 C5 C10 C9 -177.37(15) . . . . ?
C4 C3 C2 C1 68.9(2) . . . . ?
C6 C5 C4 O3 -175.14(14) . . . . ?
C6 C5 C4 C3 4.6(2) . . . . ?
C6 C5 C10 C9 1.5(2) . . . . ?
C6 C7 C8 C9 1.1(3) . . . . ?
C10 C5 C4 O3 3.7(2) . . . . ?
C10 C5 C4 C3 -176.61(15) . . . . ?
C10 C5 C6 C7 -0.7(2) . . . . ?
C7 C8 C9 C10 -0.3(3) . . . . ?
loop_
_exptl_oxdiff_crystal_face_indexfrac_h
_exptl_oxdiff_crystal_face_indexfrac_k
_exptl_oxdiff_crystal_face_indexfrac_l
_exptl_oxdiff_crystal_face_x
_exptl_oxdiff_crystal_face_y
_exptl_oxdiff_crystal_face_z
2.2697 -3.2284 -2.3420 0.5031 0.1479 -0.8515
-2.3388 3.2323 2.1703 -0.5228 -0.1538 0.8384
2.7162 0.0036 7.1459 0.7827 0.2335 0.5770
-2.7295 0.0141 -7.1354 -0.7857 -0.2344 -0.5725
-7.1527 -0.0837 7.4248 0.2677 -0.8992 0.3462
7.1527 0.0837 -7.4248 -0.2677 0.8992 -0.3462
